Tensile Strength
Get Tensile Strength essential facts below. View Videos or join the Tensile Strength discussion. Add Tensile Strength to your PopFlock.com topic list for future reference or share this resource on social media.
Tensile Strength

Two vises apply tension to a specimen by pulling at it, stretching the specimen until it fractures. The maximum stress it withstands before fracturing is its ultimate tensile strength.

Ultimate tensile strength (UTS), often shortened to tensile strength (TS), ultimate strength, or ${\displaystyle F_{\text{tu}}}$ within equations,[1][2][3] is the maximum stress that a material can withstand while being stretched or pulled before breaking. In brittle materials the ultimate tensile strength is close to the yield point, whereas in ductile materials the ultimate tensile strength can be higher.

The ultimate tensile strength is usually found by performing a tensile test and recording the engineering stress versus strain. The highest point of the stress-strain curve is the ultimate tensile strength and has units of stress.

Tensile strengths are rarely used in the design of ductile members, but they are important in brittle members. They are tabulated for common materials such as alloys, composite materials, ceramics, plastics, and wood.

## Definition

The ultimate tensile strength of a material is an intensive property; therefore its value does not depend on the size of the test specimen. However, depending on the material, it may be dependent on other factors, such as the preparation of the specimen, the presence or otherwise of surface defects, and the temperature of the test environment and material.

Some materials break very sharply, without plastic deformation, in what is called a brittle failure. Others, which are more ductile, including most metals, experience some plastic deformation and possibly necking before fracture.

Tensile strength is defined as a stress, which is measured as force per unit area. For some non-homogeneous materials (or for assembled components) it can be reported just as a force or as a force per unit width. In the International System of Units (SI), the unit is the pascal (Pa) (or a multiple thereof, often megapascals (MPa), using the SI prefix mega); or, equivalently to pascals, newtons per square metre (N/m²). A United States customary unit is pounds per square inch (lb/in² or psi), or kilo-pounds per square inch (ksi, or sometimes kpsi), which is equal to 1000 psi; kilo-pounds per square inch are commonly used in one country (US), when measuring tensile strengths.

### Ductile materials

figure 1: "Engineering" stress-strain (?-?) curve typical of aluminum
1. Ultimate strength
2. Yield strength
3. Proportional limit stress
4. Fracture
5. Offset strain (typically 0.2%)
figure 2: "Engineering" (red) and "true" (blue) stress-strain curve typical of structural steel.

Many materials can display linear elastic behavior, defined by a linear stress-strain relationship, as shown in figure 1 up to point 3. The elastic behavior of materials often extends into a non-linear region, represented in figure 1 by point 2 (the "yield point"), up to which deformations are completely recoverable upon removal of the load; that is, a specimen loaded elastically in tension will elongate, but will return to its original shape and size when unloaded. Beyond this elastic region, for ductile materials, such as steel, deformations are plastic. A plastically deformed specimen does not completely return to its original size and shape when unloaded. For many applications, plastic deformation is unacceptable, and is used as the design limitation.

After the yield point, ductile metals undergo a period of strain hardening, in which the stress increases again with increasing strain, and they begin to neck, as the cross-sectional area of the specimen decreases due to plastic flow. In a sufficiently ductile material, when necking becomes substantial, it causes a reversal of the engineering stress-strain curve (curve A, figure 2); this is because the engineering stress is calculated assuming the original cross-sectional area before necking. The reversal point is the maximum stress on the engineering stress-strain curve, and the engineering stress coordinate of this point is the ultimate tensile strength, given by point 1.

Ultimate tensile strength is not used in the design of ductile static members because design practices dictate the use of the yield stress. It is, however, used for quality control, because of the ease of testing. It is also used to roughly determine material types for unknown samples.[4]

The ultimate tensile strength is a common engineering parameter to design members made of brittle material because such materials have no yield point.[4]

## Testing

Round bar specimen after tensile stress testing
Aluminium tensile test samples after breakage
The "cup" side of the "cup-cone" characteristic failure pattern
Some parts showing the "cup" shape and some showing the "cone" shape

Typically, the testing involves taking a small sample with a fixed cross-sectional area, and then pulling it with a tensometer at a constant strain (change in gauge length divided by initial gauge length) rate until the sample breaks.

When testing some metals, indentation hardness correlates linearly with tensile strength. This important relation permits economically important nondestructive testing of bulk metal deliveries with lightweight, even portable equipment, such as hand-held Rockwell hardness testers.[5] This practical correlation helps quality assurance in metalworking industries to extend well beyond the laboratory and universal testing machines.

## Typical tensile strengths

Typical tensile strengths of some materials
Material Yield strength
(MPa)
Ultimate tensile strength
(MPa)
Density
(g/cm³)
Steel, structural ASTM A36 steel 250 400-550 7.8
Steel, 1090 mild 247 841 7.58
Chromium-vanadium steel AISI 6150 620 940 7.8
Steel, 2800 Maraging steel[6] 2617 2693 8.00
Steel, AerMet 340[7] 2160 2430 7.86
Steel, Sandvik Sanicro 36Mo logging cable precision wire[8] 1758 2070 8.00
Steel, AISI 4130, water quenched 855 °C (1570 °F), 480 °C (900 °F) temper[9] 951 1110 7.85
Steel, API 5L X65[10] 448 531 7.8
Steel, high strength alloy ASTM A514 690 760 7.8
Acrylic, clear cast sheet (PMMA)[11] 72 87[12] 1.16
High-density polyethylene (HDPE) 26-33 37 0.85
Polypropylene 12-43 19.7-80 0.91
Steel, stainless AISI 302 - cold-rolled 520[] 860 8.19
Cast iron 4.5% C, ASTM A-48 130 200 7.3
"Liquidmetal" alloy[] 1723 550-1600 6.1
Beryllium[13] 99.9% Be 345 448 1.84
Aluminium alloy[14] 2014-T6 414 483 2.8
Polyester resin (unreinforced)[15] 55 55
Polyester and chopped strand mat laminate 30% E-glass[15] 100 100
S-Glass epoxy composite[16] 2358 2358
Aluminium alloy 6061-T6 241 300 2.7
Copper 99.9% Cu 70 220[] 8.92
Cupronickel 10% Ni, 1.6% Fe, 1% Mn, balance Cu 130 350 8.94
Brass 200 + 500 8.73
Tungsten 941 1510 19.25
Glass   33[17] 2.53
E-Glass N/A 1500 for laminates,
3450 for fibers alone
2.57
S-Glass N/A 4710 2.48
Basalt fiber[18] N/A 4840 2.7
Marble N/A 15 2.6
Concrete N/A 2-5 2.7
Carbon fiber N/A 1600 for laminates,
4137 for fibers alone
1.75
Carbon fiber (Toray T1100G)[19] (the strongest human-made fibres)   7000 fibre alone 1.79
Human hair 140-160 200-250[20]
Bamboo   350-500 0.4
Spider silk (see note below) 1000 1.3
Spider silk, Darwin's bark spider[21] 1652
Silkworm silk 500   1.3
Aramid (Kevlar or Twaron) 3620 3757 1.44
UHMWPE[22] 24 52 0.97
UHMWPE fibers[23][24] (Dyneema or Spectra) 2300-3500 0.97
Vectran   2850-3340
Polybenzoxazole (Zylon)[25] 2700 5800 1.56
Wood, pine (parallel to grain)   40
Bone (limb) 104-121 130 1.6
Nylon, molded, type 6/6 450 750 1.15
Nylon fiber, drawn[26] 900[27] 1.13
Rubber - 16
Boron N/A 3100 2.46
Silicon, monocrystalline (m-Si) N/A 7000 2.33
Ultra-pure silica glass fiber-optic strands[29] 4100
Sapphire (Al2O3) 400 at 25 °C, 275 at 500 °C, 345 at 1000 °C 1900 3.9-4.1
Boron nitride nanotube N/A 33000 2.62[30]
Diamond 1600 2800 3.5
Graphene N/A intrinsic 130000;[31] engineering 50000-60000[32] 1.0
First carbon nanotube ropes ? 3600 1.3
Carbon nanotube (see note below) N/A 11000-63000 0.037-1.34
Carbon nanotube composites N/A 1200[33] N/A
High-strength carbon nanotube film N/A 9600[34] N/A
Iron (pure mono-crystal) 3 7.874
Limpet Patella vulgata teeth (Goethite) 4900
3000-6500[35]
^a Many of the values depend on manufacturing process and purity or composition.
^b Multiwalled carbon nanotubes have the highest tensile strength of any material yet measured, with one measurement of 63 GPa, still well below one theoretical value of 300 GPa.[36] The first nanotube ropes (20 mm in length) whose tensile strength was published (in 2000) had a strength of 3.6 GPa.[37] The density depends on the manufacturing method, and the lowest value is 0.037 or 0.55 (solid).[38]
^c The strength of spider silk is highly variable. It depends on many factors including kind of silk (Every spider can produce several for sundry purposes.), species, age of silk, temperature, humidity, swiftness at which stress is applied during testing, length stress is applied, and way the silk is gathered (forced silking or natural spinning).[39] The value shown in the table, 1000 MPa, is roughly representative of the results from a few studies involving several different species of spider however specific results varied greatly.[40]
^d Human hair strength varies by ethnicity and chemical treatments.
Typical properties for annealed elements[41]
Element Young's
modulus
(GPa)
Offset or
yield strength
(MPa)
Ultimate
strength
(MPa)
silicon 107 5000-9000
tungsten 411 550 550-620
iron 211 80-100 350
titanium 120 100-225 246-370
copper 130 117 210
tantalum 186 180 200
tin 47 9-14 15-200
zinc alloy 85-105 200-400 200-400
nickel 170 140-350 140-195
silver 83 170
gold 79 100
aluminium 70 15-20 40-50

## References

1. ^ "Generic MMPDS Mechanical Properties Table". stressebook.com. 6 December 2014. Archived from the original on 1 December 2017. Retrieved 2018.
2. ^ Degarmo, Black & Kohser 2003, p. 31
3. ^ Smith & Hashemi 2006, p. 223
4. ^ a b "Tensile Properties". Archived from the original on 16 February 2014. Retrieved 2015.
5. ^ E.J. Pavlina and C.J. Van Tyne, "Correlation of Yield Strength and Tensile Strength with Hardness for Steels", Journal of Materials Engineering and Performance, 17:6 (December 2008)
6. ^ "MatWeb - The Online Materials Information Resource". Archived from the original on 15 December 2013. Retrieved 2015.
7. ^ "MatWeb - The Online Materials Information Resource". Archived from the original on 21 February 2015. Retrieved 2015.
8. ^ "MatWeb - The Online Materials Information Resource". Archived from the original on 21 February 2015. Retrieved 2015.
9. ^ "MatWeb - The Online Materials Information Resource". Archived from the original on 28 March 2017. Retrieved 2015.
10. ^ "USStubular.com". Archived from the original on 13 July 2009. Retrieved 2009.
11. ^ [1] Archived 23 March 2014 at the Wayback MachineIAPD Typical Properties of Acrylics
12. ^ strictly speaking this figure is the flexural strength (or modulus of rupture), which is a more appropriate measure for brittle materials than "ultimate strength."
13. ^ "MatWeb - The Online Materials Information Resource". Archived from the original on 21 February 2015. Retrieved 2015.
14. ^ "MatWeb - The Online Materials Information Resource". Archived from the original on 21 February 2015. Retrieved 2015.
15. ^ a b "Guide to Glass Reinforced Plastic (fibreglass) - East Coast Fibreglass Supplies". Archived from the original on 16 February 2015. Retrieved 2015.
16. ^ "Properties of Carbon Fiber Tubes". Archived from the original on 24 February 2015. Retrieved 2015.
17. ^ "Soda-Lime (Float) Glass Material Properties :: MakeItFrom.com". Archived from the original on 3 July 2011. Retrieved 2015.
18. ^ "Basalt Continuous Fibers". Archived from the original on 3 November 2009. Retrieved 2009.
19. ^ "Toray Properties Document". Retrieved 2018.
20. ^ "Tensile Testing Hair". instron.us. Archived from the original on 28 September 2017.
21. ^ Agnarsson, I; Kuntner, M; Blackledge, TA (2010). "Bioprospecting Finds the Toughest Biological Material: Extraordinary Silk from a Giant Riverine Orb Spider". PLOS ONE. 5 (9): e11234. Bibcode:2010PLoSO...511234A. doi:10.1371/journal.pone.0011234. PMC 2939878. PMID 20856804.
22. ^ Oral, E; Christensen, SD; Malhi, AS; Wannomae, KK; Muratoglu, OK (2006). "PubMed Central, Table 3". J Arthroplasty. 21 (4): 580-91. doi:10.1016/j.arth.2005.07.009. PMC 2716092. PMID 16781413.
23. ^ "Tensile and creep properties of ultra high molecular weight PE fibres" (PDF). Archived from the original (PDF) on 28 June 2007. Retrieved 2007.
24. ^ "Mechanical Properties Data". www.mse.mtu.edu. Archived from the original on 3 May 2007.
25. ^ "MatWeb - The Online Materials Information Resource". Archived from the original on 21 February 2015. Retrieved 2015.
26. ^ "Nylon Fibers". University of Tennessee. Archived from the original on 19 April 2015. Retrieved 2015.
27. ^ "Comparing aramids". Teijin Aramid. Archived from the original on 3 May 2015.
28. ^ "Uhu endfest 300 epoxy: Strength over setting temperature". Archived from the original on 19 July 2011.
29. ^ "Fols.org" (PDF). Archived from the original (PDF) on 25 July 2011. Retrieved 2010.
30. ^ "What is the density of Hydrogenated Boron Nitride Nanotubes (H-BNNT)?". space.stackexchange.com. Archived from the original on 13 April 2017.
31. ^ Lee, C.; et al. (2008). "Measurement of the Elastic Properties and Intrinsic Strength of Monolayer Graphene". Science. 321 (5887): 385-8. Bibcode:2008Sci...321..385L. doi:10.1126/science.1157996. PMID 18635798. S2CID 206512830. Archived from the original on 19 February 2009. Lay summary.
32. ^ Cao, K. (2020). "Elastic straining of free-standing monolayer graphene". Nature Communications. 11 (284): 284. doi:10.1038/s41467-019-14130-0. PMC 6962388. PMID 31941941.
33. ^ IOP.org Z. Wang, P. Ciselli and T. Peijs, Nanotechnology 18, 455709, 2007.
34. ^ Xu, Wei; Chen, Yun; Zhan, Hang; Nong Wang, Jian (2016). "High-Strength Carbon Nanotube Film from Improving Alignment and Densification". Nano Letters. 16 (2): 946-952. Bibcode:2016NanoL..16..946X. doi:10.1021/acs.nanolett.5b03863. PMID 26757031.
35. ^ Barber, A. H.; Lu, D.; Pugno, N. M. (2015). "Extreme strength observed in limpet teeth". Journal of the Royal Society Interface. 12 (105): 105. doi:10.1098/rsif.2014.1326. PMC 4387522. PMID 25694539.
36. ^ Yu, Min-Feng; Lourie, O; Dyer, MJ; Moloni, K; Kelly, TF; Ruoff, RS (2000). "Strength and Breaking Mechanism of Multiwalled Carbon Nanotubes Under Tensile Load". Science. 287 (5453): 637-640. Bibcode:2000Sci...287..637Y. doi:10.1126/science.287.5453.637. PMID 10649994.
37. ^ Li, F.; Cheng, H. M.; Bai, S.; Su, G.; Dresselhaus, M. S. (2000). "Tensile strength of single-walled carbon nanotubes directly measured from their macroscopic ropes". Applied Physics Letters. 77 (20): 3161. Bibcode:2000ApPhL..77.3161L. doi:10.1063/1.1324984. Archived from the original on 28 December 2012.
38. ^ K.Hata. "From Highly Efficient Impurity-Free CNT Synthesis to DWNT forests, CNTsolids and Super-Capacitors" (PDF). Archived (PDF) from the original on 12 June 2010.
39. ^ Elices; et al. "Finding Inspiration in Argiope Trifasciata Spider Silk Fibers". JOM. Archived from the original on 15 January 2009. Retrieved 2009.
40. ^ Blackledge; et al. "Quasistatic and continuous dynamic characterization of the mechanical properties of silk from the cobweb of the black widow spider Latrodectus hesperus". The Company of Biologists. Archived from the original on 1 February 2009. Retrieved 2009.
41. ^ A.M. Howatson, P. G. Lund, and J. D. Todd, Engineering Tables and Data, p. 41